Structure of Polyvinylpyrrolidone-Iodine(Povidone-Iodine)
HANSUWE SCHENCK”, PETR SIMAK, and ERICH HAEDICKE Received April 2,1979,from the Plastics Laboratory, BASF Aktiengesellschaft, D 6700 Ludwigshafen, Federal Republic of Germany. Accepted for publication June 7,1979.
postulated (@-lo). Abstract 0 Hydrogen triiodide adducta were prepared from N,N- dimethylacetamide, N-alkylpyrrolidone derivatives, and polyvinylpyr- PVP (i - 1) 12 + Ip c4 PVP (i.12) (outer complex) rolidone, and their structures were investigated by IR spectra and X-ray s (PVP.I,/2)”2+ (Isi/2)~’2- (inner complex) structure analyses and compared with the structure of povidone-iodine - USP. The results suggest that the iodine in povidone-iodine USP is Scheme I complexed by the polymer such that a proton is fixed uia a short hydrogen The influence of the iodide ion on iodine bonding to polyvinylpyrrol- bond between two carbonyl groups of two pyrrolidone rings and that a idone in chloroform and water waa investigated (11-17). Molecular iodine triiodide anion is bound ionically to this cation. was bonded to polyvinytpyrrolidone in chloroform (18). In aqueous so- lution in the presence of potassium iodide, the polymer-bonded species Keyphrases Povidone-iodine-structure, hydrogen triiodide adducte, IR spectra, X-ray structure analysis Anti-infectives, topical-povi- was triiodide, with the potassium ion complexed directly so that an in- done-iodine, structure, hydrogen triiodide adducts, spectra, X-ray soluble product was precipitated from solution. IK The literature provides few details of the solid polyvinylpyrrolidone- structure analysis Models, molecular-povidone-iodine iodine structure. The only existing reference (19)concerns the structure of polyvinylpymolidone-iodineobtained by heating polyvinylpyrrolidone Povidone-iodine has been used as a multivalent, local, containing 10% water with iodine at 60’ for 24 hr. According to the ratio broad-spectrum antiseptic having bactericidal, fungicidal, of polyvinylpyrrolidone to iodine, some of the iodine was no longer ti- tratable with thiosulfate. The greater the ratio, the higher was the molar sporicidal, protocidal, and virucidal properties. Based on polyvinylpyrrolidone excess. On extrapolation to an infinitely large the observation that combining iodine with polyvinyl- polymer excess, 38.3% of the iodine was calculated to be present after pyrrolidone (PVP) reduces iodine vapor pressure and in- complexation in a form that was not titratable with thiosulfate. creases iodine solubility in water (l),methods were pat- Moreover, water was involved in the reaction of iodine and poly- ented that provide adduct vinylpyrrolidone; 7.4 f 3.8 moles of water was lost per mole of nontitra- a polyvinylpyrrolidone-iodine table iodine and 2.33 f 0.16 moles of acid was liberated per mole of (povidone-iodine USP). Its aqueous solution has a higher nontitratable iodine. The UV-visible spectra revealed that triiodide ions stability in storage (smaller loss of available thiosulfate- were present. titratable iodine) than an iodine solution in water con- To explain the amount of triiodide and protons formed, the decrease taining polyvinylpyrrolidone. in the amount of water, and the residual iodine, previous investigators (19) assumed that the iodine hydrolysis reaction (Scheme 11):
BACKGROUND I2 + HzO i=10- + I- + 2H+ Scheme I1 A conventional method of preparing powdered povidone-iodine in- volves efficient mixing of elemental iodine with powdered polyvinyl- is favored greatly by the presence of polyvinylpyrrolidone so that an io- pyrrolidone’. The mixture is heated at an elevated temperature until the dine complex, PVP-(12)x(IO-, I-)>, y/x < 1.5, results in which iodide and ratio of thiosulfate-titratable iodine to iodide ions is -2:l (2.3). Only this hypoiodite are present in addition to iodine. Similarly, Takikawa ut a1 ratio of iodine to iodide ions ensures adequate povidone-iodine stability. (20,21)postulated accelerated iodine hydrolysis in aqueous solution in Stability is defined as: (a) a low iodine loss as determined in a 10% the presence of polyvinylpyrrolidone and complexation to the polymer aqueous povidone-iodine solution, and (b) a high iodine distribution of the triiodide ion made up of iodide and nonhydrolyzed iodine. coefficient, cidins in water/cidi, in n-heptane, between an aqueous phaee The normal iodine hydrolysis equilibrium constant is Kw = 5.4 X 10-13 and an n-heptane phase. (22). Such an extreme shift of the iodine hydrolysis equilibrium by The distribution coefficient is the quotient of the iodine concentrations polyvinylpyrrolidone seems unlikely. Rather, it was assumed that heating in water and in n-heptane as obtained according to a literature method a mixture containing -8.3 mole % of iodine/mole (based on monomer) (4) on extracting iodine from an aqueous povidone-iodine solution with of polyvinylpyrrolidone containing 1-570 (w/w) water [the ratio typical n-heptane. Povidone-iodine also may be obtained without heating by of povidone-iodine containing 10% (w/w) active iodine] reduced iodine mixing iodine with polyvinylpyrrolidone’ and an iodide-containing to iodide with hydrogen iodide formation until, after reduction of one- substance at room temperature or by drying an iodide-containing poly- third of the iodine amount used, a stable hydrogen triiodide-polyvinyl- vinylpyrrolidone’ solution and mixing the polyvinylpyrrolidone-iodide pyrrolidone complex was present. The formation of 2 moles 01 acid/mole with iodine (5). of nontitratable iodine cwld be explained by hydrogen itdide formation In addition to the patent literature, numerous publications have dealt with hydrolysis of an intermediate iodized compound (Scheme 111): with the polyvinylpyrrolidone-iodinestructure. The term polyvinyl- RH I2+ ROH pyrrolidone-iodine has been used both for the product obtained by an- + HzO -. + 21-+ 2Hf nealing iodine with polyvinylpyrrolidone at an elevated temperature and Scheme 111 for the adduct formed on dissolving iodine in water containing this The iodine could have oxidized impurities or end groups (RH)in the polymer. The papers discussed investigations into the structure of iodine polyvinylpyrrolidone in small amounts (4.028equivalent/mole (based adducb of natural and other synthetic polymers. un monomer) of polymer in commercial povidone-iodine]. A comprehensive review article, published in 1953,dealt with numerous To confirm this hypothesis, some well-defined crystalline adducts of polyvinylpyrrolidone complexes and mentioned the adsorptivity of the lig2 - HI3 type were prepared as models of povidone-iodine materials. polyvinylpyrrolidone for iodine (6).The IR spectra were interpreted as The ligands (lig) included N,N-dimethylacetamide, N-alkylpyrrolidones, suggesting that iodine molecules, triiodide ions, and adducta of poly- and 1,3-bis(2’-pyrrolidinon-l’-yl)butane(11, a section of a polyvinyl- vinylpyrrolidone and iodine coexist. Furthermore, strong polarization pyrrolidone chain with the structure: of the iodine molecules in the adduct was inferred from the direction of dissociation of the iodine molecule as discussed recently (Scheme I) (7). Disproportionation of the iodine into hypoiodite and iodide also was
According to the USP definition for povidone.
002235491 791 1200- 1505$0 1.001 0 Journal of Pharmaceutical Sclences I 1505 @ 1979, Amricen phamceutical Association Vol. 68, No. 12. December 1979 The resultant complexes were identified structurally and compared by I. IR spectroscopy with the analogous hydrogen triiodide adduct of poly- vinylpyrrolidone prepared from polyvinylpyrrolidone, hydrogen iodide, and iodine and with polyvinylpyrrolidone-iodineor povidone-iodine obtained by annealing polyvinylpyrrolidone or povidone with iodine. Both a low (M, - 1000) and a high (M, - 10,000) molecular weight product (povidone USP) were used to analyze bonding in compounds having one or two pyrrotidnne rings, oligomers having about nine pyr- rolidone rings (polyvinylpyrrolidone of R, - lOOO), and polymers having -90 pyrrolidone rings (R,- 10,000).
Preparation of (N,N-Dimethylacetamide)2* Hydrogen Triiodide (1)-To a solution of 33.84 g (133 mmoles) of iodine in 34.84 g (400 mmoles) of N,N-dimethylacetamide was added dropwise at room tem- perature 24.32 g (133 mmoles) of hydrogen iodide as a 70%aqueous so- lution. The mixture was well stirred and cooled throughout the addition. Then the solution was diluted with 200 ml of methylene chloride and was added to 6000 ml of n-hexane. A dark solid precipitated and was filtered. The residue was washed with n-hexane and dried in uacuo to give 69.7 g (94%yield) of I as a dark solid (mp 79'). Recrystallization from meth- anol gave 53.5 g (72%yield) of I as dark-brown crystals (mp 81'). And-Calc. for C8H1913N203: C, 17.3; H, 3.4; I-, 22.9; Io, 45.8; N, 5.04. Found: C, 17.4; H, 3.6; I-, 22.6; In, 45.9; N, 5.1. Other hydrogen triiodide adducts were prepared similarly. (N-Methylpyrrolidone)2 - Hydrogen Triiodide (11)-Compound I1 formed dark red-brown crystals, mp 72-74O, in a 72% yield. The IR spectrum is shown in Fig. 1. The structure was identified by X-ray structure analysis (25) (Figs. 2 and 3). Anal.-Calc. for C10HlgT3N203:.C,20.7; H, 3.3; I,, 65.6 In, 43.8; N, 4.8. 4000 3000 2000 1600 1200 800 400 Found: C, 20.9; H, 3.2; I,, 65.7; I", 44.3; N, 4.8. 3500 2500 1800 1400 1000 600 (N-/sopropylpyrrolidone)2- Hydrogen Triiodide (Ill)-Compound CENTIMETERS-' I11 formed dark-red-brown crystals, mp 108-110', in a 23%yield. Figure 1-IR spectra of N-methylpyrrolidone (Ila),1,3-bis(2'-pyrro- Anal.-Calc. for CldH27I~N202:C, 26.4; H, 4.3; I,, 55.9; Io, 39.9; N, 4.4. lidinon-1'-y1)butane (Va), polyvinylpyrrolidone with Mn - loo0 (Vla), Found: C, 26.6; H, 4.1; I,, 59.5; I", 39.8; N, 4.8. (N-methylpyrro1idone)z - hydrogen triiodide (Il), [1,3-bis(2'-pyrroli- (N-sec-Rutylpyrrolidone)Z- Hydrogen Triiodide (IV)-Compound dinon-1'-yl)butane] hydrogen triiodide (V), and [(C&gNO)2 - H13]-5 IV formed a brown powder, mp 87-88O, in a 99%yield. (VI) based on polyvinylpyrrolidone with mn- 1000. Anal.-Calc. for CL~H~LI~N~O~:C, 28.9; H, 4.7; I3,57.3;lo, 38.2; N, 4.2. Found: C, 29.2; H, 4.7; I,, 56.8; In, 39.1; N, 4.2. Preparation of [ 1,3-Bis(2'-pyrrolidinon-l'-yl)butane] * Hydrogen as follows. Polyvinylpyrrolidone? (calc. loo%),11.1 g (0.1 mole based on Triiodide (V)-To a cooled and well-stirred solution of 12.7 g (50 monomer), was dissolved in 400 ml of analytical grade methanol, and 9.14 mmoles) of iodine and 11.2 g (50 mmoles) of 1,3-his(2'-pyrrolidinon-l'- g of 7Wo aqueous hydrogen iodide solution (0.05 mole) was added. Iodine, yl)butane in 45 ml of methylene chloride was added dropwise at room 12.7 g (0.05 mole), dissolved in 250 ml of analytical grade methylene temperature 9.14 g (50 mmoles) of hydrogen iodide as a 70% aqueous chloride, was dripped slowly into the solution; a homogeneous, slightly solution. The solution was added to 1.5 liters of n-hexane, and 29.9 g of turbid solution was obtained. The solvents were distilled off in uacuo in V precipitated as a red-violet powder (98.5%yield, mp 128'). Recrys- a rotary evaporator (540'). The resultant solid was dried over phos- tallization afforded red-brown crystals (mp 136'). The IR spectrum is phorus pentoxide to constant weight in a vacuum desiccator. shown in Figs. 1 and 4. The product (VI), a black-brown powder, was sparingly soluble in And-Calc. for C12Hp&N202: C, 23.7; H, 3.5; I;, 62.7; In, 41.8; N, 4.6. water. Its IR spectrum is shown in Figs. 1 and 4. Found: C, 24.2; H, 3.6; 1;,62.7; I", 42.2; N.4.8. Anal.-Calc. for (C12H&NO),: C, 23.8; Itod, 63.0; I,, 63.0; I-, 42.0; Preparation of Polyvinylpyrrolidone Hydrogen Triiodide Adduct N, 4.6. Found: C, 24.6; Itoh], 59.5; I;, 57.8; I-, 40.7; N, 4.4. [(C~HSNO)~* HI3l-s (V1)-The direct synthesis of VI was performed Preparation of Polyvinylpyrrolidone Hydrogen Triiodide Adduct
Melting points are uncorrected. IR spectra of the solid crystalline samples were recorded on potassium brnmide pellets (1-2 mg of substance/300 mg of potassium hrumide), while liquid samples were measured as thin films between potassium hromide disks or in thin cells. Spectra were taken with a Perkin-Elmer spectrometer. model 521 or 325. or a Digilab FTIR B/D-15. The absorptions discussed in the text and figures are in reciprocal centimeters. Microanalyses were run by the analytical laboratory of BASF Aktiengesellschaft. Iodine tbisublimed), hydrogen iodide, and potassium iodide were obtained from E. Merck, Darmstadt, West Germany, and were reagent grade. N,N-Dimethyl- arrtamide and the N-alkylpyrrolidones were obtained from BASF Aktiengesell- schaft. Ludwigshafen, West Germany, and distilled before use (purity > 99.0%by GLC). Reagent grade methylene rhloride, methanol, and n-hexane were used as solvents as supplied hy E. Merck. 1,3-Bis(2'-pyrrolidinon-l'-yl)butane was obtained by a literature method (23) from N-vinylpyrrolidone by dimerizatinn and hydrogenation. The product was pure both analytically and by GLC (>99.0%) on distillation in a spinning band column. The low molecular weight polyvinylpyrrolidone was obtained by free radical golymerization [Mn- 1O00, Mu- 2500, -2% (w/w) water] and was used as supplied y BASF Aktiengesellschaft without further urification. Hli The high molecular weight olyvinylpyrroidone was obtained by free-radical 2 eo polymerization nn- lO,oOO, bu- 40,000, -2.1% (w/w) water] and was used as supplied by BAAF Aktiengesellschaft without further purification. It met the USP requirements for povidone. Figure 2-Mean bond lengths and angles in 11. The povidone-iodine distribution coefficient was determined by a literature methnd (4).The decrease in available iodine on heat storage (15 hr, SO0) of a 10% aqueous povidone-iodine solution was determined according to USP XIX by a ~~~ ~ method similar tn that described in the literature (24). - 1o00, mu- 2500, -2% water.
1506 I Journal of Pharmaceutical Sciences Vol. 68, No. 12, December 1979 790
-*A Figure 3-Structure of I1 determined by X-ray strueture analysis: alb project ion.
* [(C&I9NO)l9.4 HIS], (Low Molecular Weight) (VII) According to 0\500' 1400 ' 1200 . 1000 900 800 700 600 500 460 Composition of Povidone-Iodine USP XIX-Method A: Direct Syn- 1500 1300 1100 thesis-P~lyvinylpyrrolidone~(calc. 100%), 111.1 g (1 mole based on WAVE NUMBER, cm-' monomer), was dissolved in 105 ml of distilled water. Then 9.4 g (0.052 Figure 5-Differential IR spectra between [(CdgNO)19.7- HIS], based mole) of 70% aqueous hydrogen iodide and 13.07 g (0.052 mole) of pow- on polyoinylpyrrolidone with m,,- lo00 (Vlla, direct synthesis; Vllb, dered iodine were added and dissolved. The solution was freeze dried, heating with iodine) and the starting polyuinylpyrrolidone. ground, and dried over phosphorus pentoxide in uacuo in a desiccator. The product (VIIa),a red-brown powder, was readily soluble in water. The distribution coefficient was 163, and the iodine loss was 22.0%. The Anal.-Calc. for (C12H&NO),,: C, 23.8; Itolal, 63.0; I;, 63.0; Io, 42.0; differential IR spectrum between VIIa and the starting polyvinylpyr- N, 4.6; acid value (stronglyacidic), 94.8. Found C, 23.4; Iwbl, 62.2; I,, 62.0; rolidone is shown in Fig. 5. Io, 45.2; N, 4.6; acid value (strongly acidic), 88.0. Anal.-Calc. for [(C6HgN0)19.4.HIa],,: C, 55.1; H+, 0.38; It,,h~,15.0; Preparation of Povidone Hydrogen Triiodide Adduct I3,15.0; I-, 10.0; N, 10.7. Found C, 52.5; H+,0.38; It,,h~,15.0; I;, 14.5; I-, [ (C&NO)l9.4 - HIS], (High Molecular Weight) (IX)(Povidone- 9.7; N, 9.5. Iodine USP X1X)-Method A: Direct Synthesis-Polyvinylpyrroli- Method B: Thermic Reaction-Poly~inylpyrrolidone~, 121g (1 mole done5 (calc. loo%), 11.1 g (0.1 mole based on monomer), was dissolved based on monomer), was mixed intimately with 19.6 g (0.0772 mole) of in 50 g of distilled water. Then 1.17 g of 55.9% (0.052 mole) aqueous hy- iodine, and the mixture was heated at 90° until no further decrease in drogen iodide and 1.31 g (0.052 mole) of iodine were added and dissolved thiosulfate-titratable iodine occurred. The product (VIIb),a red-brown by stirring for 10 hr at 50°. The solution was freeze dried, ground, and powder, was readily soluble in water. dried in a desiccator over phosphorus pentoxide. Compound IXa formed The distribution coefficient was 189, and the iodine loss was 18.2%. The as a brown, water-soluble powder. differential IR spectrum between VIIb and the starting-. polyvinylpyr- . .~ The distribution coefficient was 243, and the iodine loss was 2.4%. The rolidone is shown in Fig. 5. differential IR spectrum between 1x0 and the starting polymer is shown Anal.-Calc. for [(C~HSNO)~~.~- HIS],: Found: C, 52.0; H+,0.40; It,,hi, in Fig. 6. 14.9 I;. 14.0 I-. 9.8 N. 9.6. Anal.-Calc. for [(C~HgN0)19.~. HIS],,: C, 55.1; Itoh], 15.0; I,, 15.0; lo, Preparation of Poly&ylpyrrolidone Hydrogen Triiodide Adduct 10.0; I-, 5.0; N, 10.7. Found: C, 55.0; Itohl, 14.8; I;, 13.5; I-, 4.5; N, [ (C&N0)2 * HIsl-45 (VII1)-The direct synthesis of VIII was ac- 11.1. complished as follows. Polyvinylpyrrolidone5(calc. lOO?"), 11.1 g (0.1 mole Method B: Thermic Reaction-P~lyvinylpyrrolidone~, 113.5 g (1 mole based on monomer), was dissolved in 800 ml of analytical grade methanol. based on monomer), was mixed intimately with 21.14 g (0.0833 mole) of Then 11.37 g of 55.9% (0.05 mole) aqueous.hydrogen iodide solution was iodine. Then the mixture was heated at 80-100° until no further decrease added with efficient stirring, and 12.7 g (0.05 mole) of iodine in 500 ml in thiosulfate-titratable iodine occurred. Compound IXb formed as a of analytical grade methanol was dripped slowly into the solution. The red-brown powder and was readily soluble in water. product was prepared as described for VI. The distribution coefficient was 229, and the iodine loss was -4.5%. Compound VIII formed as a black-brown powder (30.2 g, 99.5% yield). Its IR spectrum is shown in Fig. 4.
1OOt P a 90: 80 m? !bfl50
ov lab0 1500 1400 1200 1000 800 600 460 o&OO' 1400 ' 1200 ' 1000 900 800 700 600 500 460 1700 1500 1300 1100 900 700 500 1500 1300 1100 WAVE NUMBER, cm-' WAVE NUMBER, cm-' Figure 4-IR spectra of polyoinylpyrrolidone with m,,- 10,000, V, VI Figure 6-Differential IR spectra between [(c($ffl0)19.4 (18) - Hf& based on polyoinylpyrrolidone with m,,- 1000, and [(C&gNO)z. based on polyvinylpyrrolidone with mn- 10,000 (IXa,direct synthesis; H1&5 (Vlll)based on polyvinylpyrrolidone with m,,- 10,OOO. IXb, heating with iodine) and the starting polyoinylpyrrolidone - 4 mm- 1o00, Hx - 2500, -8% water. n, - 10,000. ma- 40,000, -2.1% water = povidone USP.
Journal of Pharmaceutical Sciences f I507 Vol. 68, No. 12, December 1979 The differential IR spectrum between IXb and the starting polyvinyl- pyrrolidone is shown in Fig. 6. AnaLCalc. for [(C6HgN0)1~.0.HI&,: C, 54.4; Itohl, 16.0; IT, 16.0; Io, 10.7; I-, 5.3; N, 10.6; acid value (strongly acidic), 23.5. Found C, 51.4; I;, 15.9; I-, 5.5; N, 10.2; acid value (strongly acidic), 30. -- RESULTS AND DISCUSSION L Well-defined crystalline ligand:! .hydrogen triiodide or ligand - hy- m - 18n drogen triiodide adducts were obtained by reaction of low molecular Figure 7-Proposed structure of povidone-iodine. weight model substances for povidone-iodine [N,N-dimethylacetamide, N-alkylpyrrolidones, and 1,2-bis(2’-pyrrolidinon-l’-yl)butane, a section of a polyvinylpyrrolidone chain] with iodine and hydrogen iodide. The their IR spectra undergoing similar changes on transition from the free compounds had characteristic IR spectra different from those of the free ligand to the hydrogen triiodide adduct. Reference is made to the IR ligands (Fig. 1).The elemental analyses were consistent with the indicated spectra (Figs. 1and 4) of the free model substances polyvinylpyrrolidone structures. and the hydrogen triiodide adducts. The structural analogy is particularly The hydrogen triiodide adducts prepared usually were soluble in evident in the complex based on polyvinylpyrrolidone of n,,- 1000. It strongly polar organic solvents such as methanol. They were only spar- is less evident, although still detectable by differential spectroscopy, in ingly water soluble and hydrolyzed with the release of iodine (iodine the complex based on polyvinylpyrrolidone of mn - 10,0007 due to the flakes, heavy iodine odor). The aqueous solutions showed a strong mineral broad bands (Figs. 5 and 6). acid reaction due to the hydrogen iodide. The adducts may be regarded Even without detailed knowledge of the origin of the absorptions, it as ligand-stabilized forms of hydrogen-- triiodide acid, which does not exist is apparent that the IR spectra of the model substances agree with the in the free form. polyvinylpyrrolidone spectrum. The differences between individual As iodophores, the compounds had a high thiosulfate-titratable iodine spectra are due almost exclusively to different alkyl groups (and methyl content (45.6% in I). The-adducts were stable for months at room tem- groups in particular). Therefore, the frequency and intensity of the vi- perature without iodine loss. Dark-red single crystals of I1 of 12cm in brations of the CN-, NC=O, and carbonyl groups and the ring are largely edge length were grown. independent of the N-alkyl side chain. The bonds in the complexes of On reaction with hydrogen iodide and iodine, 1,3-bis(2’-pyrrolidi- the model substances and in the corresponding polyvinylpyrrolidone non- 1’-yl)butane yielded an adduct of the stoichiometry [ 1,3-bis(2’- adducts must be at least very similar. This view may be confirmed by pyrrolidinon-1’-yl)butane].hydrogen triiodide and not R [1,3-bis(2’- comparing IR spectra of model substances with those of the polyvinyl- pyrrolidinon-l’-yl)butane]:! hydrogen triiodide gdduct. The same adduct pyrrolidone hydrogen triiodide adducts. was obtained when using excess ligand. The ligand:! - hydrogen triiodide While there have been numerous IR spectroscopic investigations into adduct was not obtained with this ligand in any experiment. polyamides and the corresponding low molecular weight compounds, few An attempt to prepare a [(CSHgN0)2 - HIS], adduct based on poly- publications have dealt with the IR spectra of alkylpyrrolidones. vinylpyrrolidone of different molecular weights (M,,- lo00 or 10,000) Therefore, bands were assigned on the basis of the known spectra of by reacting 2 moles (based on monomer) of polymer with 1.mole of iodine N,N-dimethylacetamide (27), N,N-dimethylacetamide-dg(281, tet- and 1 mole of hydrogen iodide resulted in the loss of minor portions of ramethylurea (29), dialkylurea (301, monoalkylurea (31), 6-valerolactam the iodine and iodide and yielded products in which the pyrrolidone rings (32). and cyclopentanol (33). Further comparisons made it possible to could not all have taken part in the complexation. Based on steric and assign the bands of the hydrogen triiodide adducts. statistical considerations, participation of all pyrrolidone rings had not Notable features in the IR spectra of the hydrogen triiodide adducts been expected. were a very broad and intense absorption at about 815 cm-’ and the high Polyvinylpyrrolidone-iodineor commercial povidone-iodine, which intensity of the band at about 560 cm-’. Compared with the spectra of USP XIX requires to contain 56.6% iodide ions and 9.0-12.0% (w/w) the starting compounds, which absorbed intensely due to the carbonyl thiosulfate-titratable iodine (In), can be prepared by reacting 1 mole groups at about 1685 cm-’, the stretching vibration of the carbonyl groups (based on monomer) of polyvinylpyrrolidone6 or povidone7 with 0.052 of the adducts was hardly detectable. It appeared as a weak, very broad mole of hydrogen iodide and 0.052 mole of iodine (VII or IX, Method A) band at 1650-1600 cm-’. Such a change in the IR spectra was attributed or by heating 1 mole (monomer based) of polyvinylpyrrolidone6 or to the bonding changes in the region of the carbonyl and O=CN groups. povidone7 with 0.083 mole of iodine (VII or IX, Method B). The two The shift in position with a simultaneous intensity decrease can be ex- methods gave products with identical color, solubility, distribution plained easily by assuming a C=OH bond, including the hydrogen atom coefficient, iodine loss, elemental analysis, and IR spectrum (Figs. 5 and of hydrogen triiodide, as detected for I1 by X-ray structure analysis (25). 6). The hydrogen bonds shift the position of the carbonyl band toward The iodine loss of the aqueous solutions of the polyvinylpyrrolidone- smaller wave numbers because the double bond of the group is weakened. iodines was -18-20% (polymer of n,,- 1000) or -2-4% (polymer of M,, Strong C-0.-H-0-C bonds were found in other classes of compounds - l0,OOO) and was independent of the preparation method. Apparently, and were investigated spectroscopically. For example, the IR and Raman every proton introduced (Method A) or formed during heating (Method spectra of compounds of the metaLH(CH$00)2 type were investigated B) readily found the pyrrolidone carbonyl groups needed for complexa- and given the following assignments of the bands for (CH3COO-H-- tion due to the large molar excess of polyvinylpyrrolidone monomer OOCCH3)Na (34): units. Unequivocal proof of the structure of the hydrogen triiodide adducts vibration of the model substances was provided by the complete X-ray structure aralysis of I1 (25). The compound crystallized in the triclinic space group &-H-O -OH ,,O-H-0 C=O P1 with two triiodide units and four N-methylpyrrolidone molecules per frequency 720 1540 1285 IRinactive 1710 asymmetric unit. The result is shown in Figs. 2 and 3. A proton was fixed intensity VS,b m - S via a short hydrogen bond between two carbonyl oxygen atoms of two S pyrrolidone rings. The large triiodide anion was coordinated ionically to this large complex cation. Similar bonds were found (26) for adducts The very broad and intense absorption at 850 cm-’ in the potassium of N,N-dimethylacetamide and hexafluorbarsenic acid or hexafluoro- hydrogen oxalate spectrum, obtained by IR measurements on single phosphoric acid. A short hydrogen bond (2.40-2.45 A) links the two crystals using polarized light, was described as another hydroxyl carbonyl oxygen atoms of two N,N-dimethylacetamide molecules stietching vibration (35). The IR spectra of the hydrogen triiodide ad- (26). ducts of polyvinylpyrrolidone (VI, VIIa, VIIb, VIII, IXa, and 1x6) (Figs. The other hydrogen triiodide adducts of the model substances (I-V) 46) showed that the carbonyl groups did not all participate in the adduct aKd the corresponding complexes prepared using polyvinylpyrrolidone formation (this was expected in view of the elemental analysis of VI and (M, - lOOO, X,, - l0,OOO) are believed to be analogous in structure, with VIII and because of the large excess of pyrrolidone rings in the VII and IX mixture). The absorptions at -800 and 1020 cm-’, characteristic of the adduct structure, occurred. ‘m - 1000 -22500. In adducts VI and VIII, these characteristic absorptions were clearly ’ - 10,060. fiW- 40,000 = povidone USP. visible. In VIla, IXa, VIIb, and IXb, which have the composition of
1508 I Journal of Pharmaceutical Sciences Vol. 68, No. 12, December 1979 commercial povidone-iodinewith an approximately 10-foldmolar excess 3,028,300 (1960). of pyrrolidone rings, these characteristic absorptions showed up in the (5) A. Cantor and M. W. Winicov (West Laboratories Inc.), German differential spectra between the starting polyvinylpyrrolidone and the pat. 2,422,767 (1974); through Chem. Abstr., 82,103138~(1975). adducts. (6) W. Scholtan, Makromol. Chem., 11,131 (1954). Contrary to conventional assumptions on the structure of polyvinyl- (7) I. Moriguchi, Y. Araki, and N. Kaneniwa, Chem. fharm. Bull., pyrrolidone-iodine prepared by heating polyvinylpyrrolidonee with io- 17,2088 (1969). dine, the compound probably is an adduct of the polymer and hydrogen (8) V. 0. Mokhnach and I,. N. Propp, Dokl. Akad. Nauk SSR, 170, triiodide in which a proton is fixed between two carbonyl groups of two 103 (1966); through Chem. Abstr., 66,60485j (1967). pyrrolidone rings (cf., Fig. 7) and the triiodide anion is bound ionically (9) V. 0. Mokhnach and I. P. Zueva, Zh. Neorgan. Khim., 8, 668 to this complex cation. Incidentally, the pyrrolidone rings participating (1963); through Chem. Abstr., 58,13304h (1963). in the complexation need not be vicinal in the polymer chain as shown (10) W. W. Korshak, L. B. Zubakova, L. Y. Nikiforova, and N. V. in Fig. 7. Due to an appreciable excess of free pyrrolidone rings in povi- Kachurina, Tr. Mosk. Khim.-Tekhnol.Inst., 1972, No. 70,201; through done-iodine USP XIX, the product was readily soluble in water. Chern. Abstr., 79,23822q (1973). (11) S. M. Barkin, H. P. Frank, and F. R. Eirich, Ric. Sci., 25, Suppl. SUMMARY Simp. Int. Chirn. Macrornol., Milan- Turin, 1954,844; through Chem. Abstr., 54,11554a (1960). N,N-Dimethylacetamide and N-alkylpyrrolidones are capable of (12) J. Ndl and B. Sbille, C. R. Hebd. Sfances Acad. Sci. Ser. C, 252, forming stable ligandn - hydrogen triiodide adducts. This finding coin- 405 (1961). cides neatly with the complex chemistry of these organic compounds (13) J. Nee1 and B. SBbille, J. Chim. Phys.-Chim. Biol., 58, 738 discussed in the literature. The bonding is similar in all adducts of this (1961). type, where a proton is fixed between two carbonyl groups of two ligands (14) G. Oster and E. H. Immergut, J. Am. Chem. Soc., 76, 1393 uia a short hydrogen bond. This bonding manifests itself in similar IR (1954). spectra of the complexes, which all show a strong shift of the carbonyl (15) N. Kaneniwa and A. Ikekawa, Chem. fharm. Bull., 22. 2990 band toward lower wave numbers. For 11, this structure could be un- (1974). equivocally verified (25). (16) F. Eirich, Chem. Eng. News,32.2768 f 1954). By analogy with the model compounds, polyvinylpyrrolidones can be (17) J. Ndl and B. S6bille~C. R. Hebd. Seances Arad. Sci. Ser. C, 252, reacted with hydrogen iodide and iodine to form adducts whose spec- 867 (1961). troscopic properties are analogous to those of the low molecular weight (18) J. Eliassaf, Eur. Polym. J., 2,269 (1966). complexes, which suggests identical bonding. However, for steric reasons, (19) R. F. Cournoyer and S. Siggia, J. folym. Sci. Polym. Chem., 12, it seems impossible for all pyrrolidone rings to take part in adduct for- 603 (1974). mation. If there is more halogen, halogen losses occur on drying. If there (20) K. Takikawa, M. Nakano, and T. Arita, Chem. Pharm. Bull., 26, are 520 pyrrolidone rings for every hydrogen triiodide, as in commercial 874 (1978). povidone-iodine, complexation is good and the excess pyrrolidone rings (21) Ibid., 26,1370 (1978). not taking part in the romplexation provide the desired water solu- . (22) T. L. Allen and R. M. Keefer, J. Am. Chem. Soc., 77, 2957 bility. (1955). The structure of povidone-iodine USP XIX prepared by heating (23) J. W. Breitenbach, F. Galinovsky, H. Nesvadba, and E. Wolf, p~lyvinylpyrrolidone~with iodine agrees with that of a product obtained Monatsh. Chem., 87,580 (1956). by the direct synthesis of p~lyvinylpyrrolidone~,hydrogen iodide, and (24) Defense Medical Purchase Description No. 4, Jan. 4, 1972, p. 4, iodine. Previous assumptions regarding the structure of polyvinylpyr- 6505-491-7557 and 6505-994-7224. rolidone-iodine (18-20) are not consistent with the results discussed in (25) H. U. Schenck, P. Simak, and E. Haedicke, Makromol. Chem., this paper. in press. (26) D. Cook, Can. J. Chem., 42,2721 (1964). REFERENCES (27) G. Durgaprasad, D. N. Sathyanarayana, C. C. Patel, H. S. Randhawa, A. Goel, and C. N. R. Rao, Spectrochim. Acta, Part A, 28, (1) H. A. Shelanski, US. pat. 2,739,922 (1956);through Chem. Abstr., 2311 (1972). 50,11623g (1956). (28)K.-L. Dorris, T. H. Sidall, W. E. Stewart, and M. L. Good, ibid., (2) H. Beller and W. A. Hosmer (General Aniline & Film Corp.), US. 23.1657 (1967). pat. 2,706,701 (1955); through Chem. Abstr., 49,12788a (1955). (29) H. Spell and J. Laane, ibid., 28.295 (1972). (3) S. Siggia (General Aniline & Film Corp.), US. pat. 2,900,305 (30) Y. Mido, ibid., 28, 1503 (1972). (1956). (31) C. I. Jose, ibid., 25,111 (1969). (4) A. Cantor and M. W. Winicov (West Laboratories Inc.), US.pat. (32) M. Rey-Lafon and M. T. Forel, ibid., 29,471 (1973). (33) J. Durig, J. M. Karriker, and W. C. Harris, ibid., 27, 1955 (1971). (34) D. Hadii, B. Orel, and A. Novak, ibid., 29,1745 (1973). - 1000, A 2500 or - 10,000. mw - 40,000. (35) B. Orel, thesis, University of Ljubljana, Yugoslavia, 1972.
Journal of pharmaceutical Sciences I 1509 Voi. 68, No. 12, December 1979